# Supplementary Information (SI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2025

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_shelx
_database_code_depnum_ccdc_archive 'CCDC 2346856'
loop_
_audit_author_name
_audit_author_address
'Wataru Hikita'
;Graduate School of Science and Technology, Niigata University
Japan
;
_audit_update_record             
;
2024-04-09 deposited with the CCDC.	2025-02-19 downloaded from the CCDC.
;

_audit_creation_date             2022-08-29T20:43:44-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.5
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic

#----------------------------------------------------------------------------#
#                   CHEMICAL INFORMATION                                     #
#----------------------------------------------------------------------------#

_chemical_formula_sum            'Ca2 Ga1.87 Mn0.13 O6 Sr'
_chemical_formula_weight         401.26
_chemical_absolute_configuration unk

#----------------------------------------------------------------------------#
#                   UNIT CELL INFORMATION                                    #
#----------------------------------------------------------------------------#

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'F 4 3 2'
_symmetry_space_group_name_Hall  'F 4 2 3'
_symmetry_Int_Tables_number      209
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'y, -x+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'x, z+1/2, -y+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'x, -z+1/2, y+1/2'
'z, y+1/2, -x+1/2'
'z, -y+1/2, x+1/2'
'-z, y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'y+1/2, -x, z+1/2'
'-y+1/2, x, z+1/2'
'x+1/2, z, -y+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'x+1/2, -z, y+1/2'
'z+1/2, y, -x+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'y+1/2, -x+1/2, z'
'-y+1/2, x+1/2, z'
'x+1/2, z+1/2, -y'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'x+1/2, -z+1/2, y'
'z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, x'
'-z+1/2, -y+1/2, -x'

_cell_length_a                   15.4894(15)
_cell_length_b                   15.4894(15)
_cell_length_c                   15.4894(15)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     3716.2(11)
_cell_formula_units_Z            24
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1992
_cell_measurement_theta_min      2.28
_cell_measurement_theta_max      27.49
_cell_measurement_wavelength     0.71073

#----------------------------------------------------------------------------#
#                   CRYSTAL INFORMATION                                      #
#----------------------------------------------------------------------------#

_exptl_crystal_description       prism
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.109
_exptl_crystal_size_mid          0.094
_exptl_crystal_size_min          0.091
_exptl_crystal_density_diffrn    4.303
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4493

#----------------------------------------------------------------------------#
#                   ABSORPTION CORRECTION                                    #
#----------------------------------------------------------------------------#

_exptl_absorpt_coefficient_mu    18.535
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'NUMABS (Rigaku, 1999)'
_exptl_absorpt_correction_T_min  1
_exptl_absorpt_correction_T_max  1
_shelx_estimated_absorpt_T_min   0.237
_shelx_estimated_absorpt_T_max   0.283

#----------------------------------------------------------------------------#
#                   DATA COLLECTION                                          #
#----------------------------------------------------------------------------#

_diffrn_source                   'sealed x-ray tube'
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 6.849
_diffrn_measurement_device_type  'Rigaku XtaLAB mini'
_diffrn_measurement_method       ω
_diffrn_standards_number         0
_diffrn_standards_interval_time  .
_diffrn_standards_interval_count .
_diffrn_standards_decay_%        ?
_diffrn_reflns_av_R_equivalents  0.056
_diffrn_reflns_av_unetI/netI     0.02
_diffrn_reflns_number            6448
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         2.277
_diffrn_reflns_theta_max         27.461
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_reflns_Laue_measured_fraction_full 1
_diffrn_reflns_Laue_measured_fraction_max 1
_diffrn_reflns_point_group_measured_fraction_full 1
_diffrn_reflns_point_group_measured_fraction_max 1
_reflns_Friedel_fraction_full    1
_reflns_Friedel_fraction_max     1
_reflns_Friedel_coverage         0.423
_reflns_number_total             377
_reflns_number_gt                377
_reflns_threshold_expression     'I > 2σ(I)'

#----------------------------------------------------------------------------#
#                   COMPUTER PROGRAMS USED                                   #
#----------------------------------------------------------------------------#

_computing_data_collection       'CrystalClear (Rigaku/MSC Inc., 2006)'
_computing_cell_refinement       'CrystalClear (Rigaku/MSC Inc., 2006)'
_computing_data_reduction        
'CrystalClear (Rigaku/MSC Inc., 2006), SORTAV (Blessing, 1995)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    'Ortep-3 for Windows (Farrugia, 2012)'
_computing_publication_material  'WinGX publication routines (Farrugia, 2012)'

#----------------------------------------------------------------------------#
#                   STRUCTURE SOLUTION                                       #
#----------------------------------------------------------------------------#


#----------------------------------------------------------------------------#
#                   REFINEMENT INFORMATION                                   #
#----------------------------------------------------------------------------#

_shelx_SHELXL_version_number     2018/3
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0214P)²+160.8083P] where P=(Fo²+2Fc²)/3'
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_coef       0.00013(3)
_refine_ls_number_reflns         377
_refine_ls_number_parameters     37
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_R_factor_all          0.0317
_refine_ls_R_factor_gt           0.0317
_refine_ls_wR_factor_ref         0.0795
_refine_ls_wR_factor_gt          0.0795
_refine_ls_goodness_of_fit_ref   1.272
_refine_ls_restrained_S_all      1.272
_refine_ls_shift/su_max          0
_refine_ls_shift/su_mean         0
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.15(8)
_refine_diff_density_max         1.248
_refine_diff_density_min         -0.709
_refine_diff_density_rms         0.169

#----------------------------------------------------------------------------#
#                   CONSTRAINTS AND RESTRAINTS                               #
#----------------------------------------------------------------------------#


#----------------------------------------------------------------------------#
#                   ATOMIC TYPES, COORDINATES AND THERMAL PARAMETERS         #
#----------------------------------------------------------------------------#

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.20879(8) 1 0 0.0134(4) Uani 1 4 d S T P . .
Ga1 Ga 0.5 1 0 0.0037(16) Uani 0.20(8) 24 d S T P . .
Mn1 Mn 0.5 1 0 0.0037(16) Uani 0.80(8) 24 d S T P . .
Ga2 Ga 0.17737(17) 0.82263(17) 0.17737(17) 0.0172(9) Uani 0.5 3 d S T P . .
Ga3 Ga 0.25 1 0.25 0.0139(4) Uani 1 4 d S T P . .
Ga4 Ga 0 1 0 0.0136(8) Uani 1 24 d S T P . .
Ca1 Ca 0.38960(8) 0.88960(8) 0.11040(8) 0.0068(5) Uani 1 3 d S T P . .
Ca2 Ca 0.1564(4) 0.8436(4) 0.1564(4) 0.031(2) Uani 0.5 3 d S T P . .
O1 O 0.3746(6) 1 0 0.0077(17) Uani 1 4 d S T P . .
O2 O 0.25 0.75 0.25 0.027(4) Uani 1 12 d S T P . .
O3 O 0.2509(6) 0.9334(6) 0.1513(4) 0.033(2) Uani 1 1 d . . . . .
O4 O 0.0681(6) 0.9319(6) 0.0681(6) 0.017(4) Uani 0.5 3 d S T P . .



#----------------------------------------------------------------------------#
#                   MOLECULAR GEOMETRY                                       #
#----------------------------------------------------------------------------#

_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 O1 2.568(9) . ?
Sr1 O4 2.6409(11) 14_665 ?
Sr1 O4 2.6409(11) . ?
Sr1 O4 2.6409(12) 4_575 ?
Sr1 O4 2.6409(12) 16_665 ?
Sr1 O3 2.643(7) 17_566 ?
Sr1 O3 2.643(7) 20_564 ?
Sr1 O3 2.643(7) 4_575 ?
Sr1 O3 2.643(7) . ?
Sr1 Ga4 3.2340(14) . ?
Sr1 Ca2 3.520(8) 14_665 ?
Sr1 Ca2 3.520(8) 16_665 ?
Ga1 O1 1.942(9) 58_665 ?
Ga1 O1 1.942(9) 57_464 ?
Ga1 O1 1.942(9) 78_566 ?
Ga1 O1 1.942(9) 77_554 ?
Ga1 O1 1.942(9) 2_675 ?
Ga1 O1 1.942(9) . ?
Ga1 Ca1 2.962(2) 85_455 ?
Ga1 Ca1 2.962(2) 2_675 ?
Ga1 Ca1 2.962(2) . ?
Ga1 Ca1 2.962(2) 88_655 ?
Ga1 Ca1 2.962(2) 4_575 ?
Ga1 Ca1 2.962(2) 3_655 ?
Mn1 O1 1.942(9) 58_665 ?
Mn1 O1 1.942(9) 57_464 ?
Mn1 O1 1.942(9) 78_566 ?
Mn1 O1 1.942(9) 77_554 ?
Mn1 O1 1.942(9) 2_675 ?
Mn1 O1 1.942(9) . ?
Mn1 Ca1 2.962(2) 85_455 ?
Mn1 Ca1 2.962(2) 2_675 ?
Mn1 Ca1 2.962(2) . ?
Mn1 Ca1 2.962(2) 88_655 ?
Mn1 Ca1 2.962(2) 4_575 ?
Mn1 Ca1 2.962(2) 3_655 ?
Ga2 O2 1.949(4) . ?
Ga2 O3 2.098(11) . ?
Ga2 O3 2.098(10) 6_566 ?
Ga2 O3 2.098(11) 12_665 ?
Ga2 Ca1 3.600(2) 74_565 ?
Ga2 Ca1 3.600(2) . ?
Ga2 Ca1 3.600(2) 51 ?
Ga2 Ca2 3.656(12) 51 ?
Ga2 Ca2 3.656(12) 74_565 ?
Ga2 Ca2 3.656(12) 28_565 ?
Ga3 O3 1.844(7) . ?
Ga3 O3 1.844(7) 72_575 ?
Ga3 O3 1.844(7) 22_575 ?
Ga3 O3 1.844(7) 51 ?
Ga3 Ca2 3.1738(11) . ?
Ga3 Ca2 3.1738(11) 61_465 ?
Ga3 Ca2 3.1738(10) 16_665 ?
Ga3 Ca2 3.1738(11) 51 ?
Ga3 Ca1 3.5036(10) 51 ?
Ga3 Ca1 3.5036(10) 87_465 ?
Ga3 Ca1 3.5036(10) 38_665 ?
Ga3 Ca1 3.5036(10) . ?
Ga4 O4 1.828(17) 16_665 ?
Ga4 O4 1.828(17) 3 ?
Ga4 O4 1.828(17) 15_465 ?
Ga4 O4 1.828(17) 14_665 ?
Ga4 O4 1.828(17) 13_465 ?
Ga4 O4 1.828(17) 4_575 ?
Ga4 O4 1.828(17) 2_575 ?
Ga4 O4 1.828(17) . ?
Ca1 O3 2.340(8) 80_556 ?
Ca1 O3 2.340(8) 59_465 ?
Ca1 O3 2.340(8) . ?
Ca1 O1 2.4296(18) 58_665 ?
Ca1 O1 2.4296(18) 77_554 ?
Ca1 O1 2.4296(18) . ?
Ca1 Ca1 3.420(2) 88_655 ?
Ca1 Ca1 3.420(2) 87_465 ?
Ca1 Ca1 3.420(2) 85_455 ?
Ca2 O3 2.021(11) . ?
Ca2 O3 2.021(11) 12_665 ?
Ca2 O3 2.021(11) 6_566 ?
Ca2 O4 2.37(2) . ?
Ca2 O2 2.512(11) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Sr1 O4 145.6(4) . 14_665 ?
O1 Sr1 O4 145.6(4) . . ?
O4 Sr1 O4 47.1(5) 14_665 . ?
O1 Sr1 O4 145.6(4) . 4_575 ?
O4 Sr1 O4 47.1(5) 14_665 4_575 ?
O4 Sr1 O4 68.8(7) . 4_575 ?
O1 Sr1 O4 145.6(4) . 16_665 ?
O4 Sr1 O4 68.8(7) 14_665 16_665 ?
O4 Sr1 O4 47.1(5) . 16_665 ?
O4 Sr1 O4 47.1(5) 4_575 16_665 ?
O1 Sr1 O3 75.7(2) . 17_566 ?
O4 Sr1 O3 135.6(4) 14_665 17_566 ?
O4 Sr1 O3 113.7(2) . 17_566 ?
O4 Sr1 O3 90.3(2) 4_575 17_566 ?
O4 Sr1 O3 72.1(4) 16_665 17_566 ?
O1 Sr1 O3 75.7(2) . 20_564 ?
O4 Sr1 O3 72.1(4) 14_665 20_564 ?
O4 Sr1 O3 90.3(2) . 20_564 ?
O4 Sr1 O3 113.7(2) 4_575 20_564 ?
O4 Sr1 O3 135.6(4) 16_665 20_564 ?
O3 Sr1 O3 151.4(4) 17_566 20_564 ?
O1 Sr1 O3 75.7(2) . 4_575 ?
O4 Sr1 O3 90.3(2) 14_665 4_575 ?
O4 Sr1 O3 135.6(4) . 4_575 ?
O4 Sr1 O3 72.1(4) 4_575 4_575 ?
O4 Sr1 O3 113.7(2) 16_665 4_575 ?
O3 Sr1 O3 86.50(10) 17_566 4_575 ?
O3 Sr1 O3 86.50(10) 20_564 4_575 ?
O1 Sr1 O3 75.7(2) . . ?
O4 Sr1 O3 113.7(2) 14_665 . ?
O4 Sr1 O3 72.1(4) . . ?
O4 Sr1 O3 135.6(4) 4_575 . ?
O4 Sr1 O3 90.3(2) 16_665 . ?
O3 Sr1 O3 86.50(10) 17_566 . ?
O3 Sr1 O3 86.50(10) 20_564 . ?
O3 Sr1 O3 151.4(4) 4_575 . ?
O1 Sr1 Ga4 180 . . ?
O4 Sr1 Ga4 34.4(4) 14_665 . ?
O4 Sr1 Ga4 34.4(4) . . ?
O4 Sr1 Ga4 34.4(4) 4_575 . ?
O4 Sr1 Ga4 34.4(4) 16_665 . ?
O3 Sr1 Ga4 104.3(2) 17_566 . ?
O3 Sr1 Ga4 104.3(2) 20_564 . ?
O3 Sr1 Ga4 104.3(2) 4_575 . ?
O3 Sr1 Ga4 104.3(2) . . ?
O1 Sr1 Ca2 103.33(14) . 14_665 ?
O4 Sr1 Ca2 42.3(4) 14_665 14_665 ?
O4 Sr1 Ca2 79.03(13) . 14_665 ?
O4 Sr1 Ca2 79.03(13) 4_575 14_665 ?
O4 Sr1 Ca2 111.1(4) 16_665 14_665 ?
O3 Sr1 Ca2 159.37(18) 17_566 14_665 ?
O3 Sr1 Ca2 34.7(3) 20_564 14_665 ?
O3 Sr1 Ca2 73.47(17) 4_575 14_665 ?
O3 Sr1 Ca2 113.48(19) . 14_665 ?
Ga4 Sr1 Ca2 76.67(14) . 14_665 ?
O1 Sr1 Ca2 103.33(14) . 16_665 ?
O4 Sr1 Ca2 111.1(4) 14_665 16_665 ?
O4 Sr1 Ca2 79.03(13) . 16_665 ?
O4 Sr1 Ca2 79.03(13) 4_575 16_665 ?
O4 Sr1 Ca2 42.3(4) 16_665 16_665 ?
O3 Sr1 Ca2 34.7(3) 17_566 16_665 ?
O3 Sr1 Ca2 159.37(18) 20_564 16_665 ?
O3 Sr1 Ca2 113.48(19) 4_575 16_665 ?
O3 Sr1 Ca2 73.47(17) . 16_665 ?
Ga4 Sr1 Ca2 76.67(14) . 16_665 ?
Ca2 Sr1 Ca2 153.3(3) 14_665 16_665 ?
O1 Ga1 O1 180 58_665 57_464 ?
O1 Ga1 O1 90 58_665 78_566 ?
O1 Ga1 O1 90 57_464 78_566 ?
O1 Ga1 O1 90 58_665 77_554 ?
O1 Ga1 O1 90 57_464 77_554 ?
O1 Ga1 O1 180 78_566 77_554 ?
O1 Ga1 O1 90.000(2) 58_665 2_675 ?
O1 Ga1 O1 90 57_464 2_675 ?
O1 Ga1 O1 90.000(2) 78_566 2_675 ?
O1 Ga1 O1 90 77_554 2_675 ?
O1 Ga1 O1 90 58_665 . ?
O1 Ga1 O1 90.000(2) 57_464 . ?
O1 Ga1 O1 90 78_566 . ?
O1 Ga1 O1 90.000(2) 77_554 . ?
O1 Ga1 O1 180 2_675 . ?
O1 Ga1 Ca1 125.2640(10) 58_665 85_455 ?
O1 Ga1 Ca1 54.7360(10) 57_464 85_455 ?
O1 Ga1 Ca1 125.2640(10) 78_566 85_455 ?
O1 Ga1 Ca1 54.7360(10) 77_554 85_455 ?
O1 Ga1 Ca1 125.3 2_675 85_455 ?
O1 Ga1 Ca1 54.7 . 85_455 ?
O1 Ga1 Ca1 54.7360(10) 58_665 2_675 ?
O1 Ga1 Ca1 125.3 57_464 2_675 ?
O1 Ga1 Ca1 54.7360(10) 78_566 2_675 ?
O1 Ga1 Ca1 125.2640(10) 77_554 2_675 ?
O1 Ga1 Ca1 54.7 2_675 2_675 ?
O1 Ga1 Ca1 125.3 . 2_675 ?
Ca1 Ga1 Ca1 180 85_455 2_675 ?
O1 Ga1 Ca1 54.7360(10) 58_665 . ?
O1 Ga1 Ca1 125.2640(10) 57_464 . ?
O1 Ga1 Ca1 125.2640(10) 78_566 . ?
O1 Ga1 Ca1 54.7360(10) 77_554 . ?
O1 Ga1 Ca1 125.3 2_675 . ?
O1 Ga1 Ca1 54.7 . . ?
Ca1 Ga1 Ca1 70.5 85_455 . ?
Ca1 Ga1 Ca1 109.5 2_675 . ?
O1 Ga1 Ca1 54.7360(10) 58_665 88_655 ?
O1 Ga1 Ca1 125.2640(10) 57_464 88_655 ?
O1 Ga1 Ca1 125.2640(10) 78_566 88_655 ?
O1 Ga1 Ca1 54.7360(10) 77_554 88_655 ?
O1 Ga1 Ca1 54.7 2_675 88_655 ?
O1 Ga1 Ca1 125.3 . 88_655 ?
Ca1 Ga1 Ca1 109.5 85_455 88_655 ?
Ca1 Ga1 Ca1 70.5 2_675 88_655 ?
Ca1 Ga1 Ca1 70.5 . 88_655 ?
O1 Ga1 Ca1 125.2640(10) 58_665 4_575 ?
O1 Ga1 Ca1 54.7360(10) 57_464 4_575 ?
O1 Ga1 Ca1 54.7360(10) 78_566 4_575 ?
O1 Ga1 Ca1 125.2640(10) 77_554 4_575 ?
O1 Ga1 Ca1 125.3 2_675 4_575 ?
O1 Ga1 Ca1 54.7 . 4_575 ?
Ca1 Ga1 Ca1 70.5 85_455 4_575 ?
Ca1 Ga1 Ca1 109.5 2_675 4_575 ?
Ca1 Ga1 Ca1 109.4710(10) . 4_575 ?
Ca1 Ga1 Ca1 180 88_655 4_575 ?
O1 Ga1 Ca1 125.2640(10) 58_665 3_655 ?
O1 Ga1 Ca1 54.7360(10) 57_464 3_655 ?
O1 Ga1 Ca1 125.2640(10) 78_566 3_655 ?
O1 Ga1 Ca1 54.7 77_554 3_655 ?
O1 Ga1 Ca1 54.7 2_675 3_655 ?
O1 Ga1 Ca1 125.3 . 3_655 ?
Ca1 Ga1 Ca1 70.5 85_455 3_655 ?
Ca1 Ga1 Ca1 109.5 2_675 3_655 ?
Ca1 Ga1 Ca1 109.5 . 3_655 ?
Ca1 Ga1 Ca1 70.5 88_655 3_655 ?
Ca1 Ga1 Ca1 109.5 4_575 3_655 ?
O1 Mn1 O1 180 58_665 57_464 ?
O1 Mn1 O1 90 58_665 78_566 ?
O1 Mn1 O1 90 57_464 78_566 ?
O1 Mn1 O1 90 58_665 77_554 ?
O1 Mn1 O1 90 57_464 77_554 ?
O1 Mn1 O1 180 78_566 77_554 ?
O1 Mn1 O1 90.000(2) 58_665 2_675 ?
O1 Mn1 O1 90 57_464 2_675 ?
O1 Mn1 O1 90.000(2) 78_566 2_675 ?
O1 Mn1 O1 90 77_554 2_675 ?
O1 Mn1 O1 90 58_665 . ?
O1 Mn1 O1 90.000(2) 57_464 . ?
O1 Mn1 O1 90 78_566 . ?
O1 Mn1 O1 90.000(2) 77_554 . ?
O1 Mn1 O1 180 2_675 . ?
O1 Mn1 Ca1 125.2640(10) 58_665 85_455 ?
O1 Mn1 Ca1 54.7360(10) 57_464 85_455 ?
O1 Mn1 Ca1 125.2640(10) 78_566 85_455 ?
O1 Mn1 Ca1 54.7360(10) 77_554 85_455 ?
O1 Mn1 Ca1 125.3 2_675 85_455 ?
O1 Mn1 Ca1 54.7 . 85_455 ?
O1 Mn1 Ca1 54.7360(10) 58_665 2_675 ?
O1 Mn1 Ca1 125.3 57_464 2_675 ?
O1 Mn1 Ca1 54.7360(10) 78_566 2_675 ?
O1 Mn1 Ca1 125.2640(10) 77_554 2_675 ?
O1 Mn1 Ca1 54.7 2_675 2_675 ?
O1 Mn1 Ca1 125.3 . 2_675 ?
Ca1 Mn1 Ca1 180 85_455 2_675 ?
O1 Mn1 Ca1 54.7360(10) 58_665 . ?
O1 Mn1 Ca1 125.2640(10) 57_464 . ?
O1 Mn1 Ca1 125.2640(10) 78_566 . ?
O1 Mn1 Ca1 54.7360(10) 77_554 . ?
O1 Mn1 Ca1 125.3 2_675 . ?
O1 Mn1 Ca1 54.7 . . ?
Ca1 Mn1 Ca1 70.5 85_455 . ?
Ca1 Mn1 Ca1 109.5 2_675 . ?
O1 Mn1 Ca1 54.7360(10) 58_665 88_655 ?
O1 Mn1 Ca1 125.2640(10) 57_464 88_655 ?
O1 Mn1 Ca1 125.2640(10) 78_566 88_655 ?
O1 Mn1 Ca1 54.7360(10) 77_554 88_655 ?
O1 Mn1 Ca1 54.7 2_675 88_655 ?
O1 Mn1 Ca1 125.3 . 88_655 ?
Ca1 Mn1 Ca1 109.5 85_455 88_655 ?
Ca1 Mn1 Ca1 70.5 2_675 88_655 ?
Ca1 Mn1 Ca1 70.5 . 88_655 ?
O1 Mn1 Ca1 125.2640(10) 58_665 4_575 ?
O1 Mn1 Ca1 54.7360(10) 57_464 4_575 ?
O1 Mn1 Ca1 54.7360(10) 78_566 4_575 ?
O1 Mn1 Ca1 125.2640(10) 77_554 4_575 ?
O1 Mn1 Ca1 125.3 2_675 4_575 ?
O1 Mn1 Ca1 54.7 . 4_575 ?
Ca1 Mn1 Ca1 70.5 85_455 4_575 ?
Ca1 Mn1 Ca1 109.5 2_675 4_575 ?
Ca1 Mn1 Ca1 109.4710(10) . 4_575 ?
Ca1 Mn1 Ca1 180 88_655 4_575 ?
O1 Mn1 Ca1 125.2640(10) 58_665 3_655 ?
O1 Mn1 Ca1 54.7360(10) 57_464 3_655 ?
O1 Mn1 Ca1 125.2640(10) 78_566 3_655 ?
O1 Mn1 Ca1 54.7 77_554 3_655 ?
O1 Mn1 Ca1 54.7 2_675 3_655 ?
O1 Mn1 Ca1 125.3 . 3_655 ?
Ca1 Mn1 Ca1 70.5 85_455 3_655 ?
Ca1 Mn1 Ca1 109.5 2_675 3_655 ?
Ca1 Mn1 Ca1 109.5 . 3_655 ?
Ca1 Mn1 Ca1 70.5 88_655 3_655 ?
Ca1 Mn1 Ca1 109.5 4_575 3_655 ?
O2 Ga2 O3 105.6(2) . . ?
O2 Ga2 O3 105.6(2) . 6_566 ?
O3 Ga2 O3 113.03(19) . 6_566 ?
O2 Ga2 O3 105.6(2) . 12_665 ?
O3 Ga2 O3 113.03(19) . 12_665 ?
O3 Ga2 O3 113.03(19) 6_566 12_665 ?
O2 Ga2 Ca1 78.78(7) . 74_565 ?
O3 Ga2 Ca1 147.95(18) . 74_565 ?
O3 Ga2 Ca1 38.1(2) 6_566 74_565 ?
O3 Ga2 Ca1 95.53(19) 12_665 74_565 ?
O2 Ga2 Ca1 78.78(7) . . ?
O3 Ga2 Ca1 38.1(2) . . ?
O3 Ga2 Ca1 95.53(19) 6_566 . ?
O3 Ga2 Ca1 147.95(19) 12_665 . ?
Ca1 Ga2 Ca1 116.31(5) 74_565 . ?
O2 Ga2 Ca1 78.78(7) . 51 ?
O3 Ga2 Ca1 95.53(18) . 51 ?
O3 Ga2 Ca1 147.95(19) 6_566 51 ?
O3 Ga2 Ca1 38.1(2) 12_665 51 ?
Ca1 Ga2 Ca1 116.31(5) 74_565 51 ?
Ca1 Ga2 Ca1 116.31(5) . 51 ?
O2 Ga2 Ca2 40.37(7) . 51 ?
O3 Ga2 Ca2 71.3(2) . 51 ?
O3 Ga2 Ca2 139.4(2) 6_566 51 ?
O3 Ga2 Ca2 100.1(2) 12_665 51 ?
Ca1 Ga2 Ca2 119.15(10) 74_565 51 ?
Ca1 Ga2 Ca2 62.24(6) . 51 ?
Ca1 Ga2 Ca2 62.24(6) 51 51 ?
O2 Ga2 Ca2 40.37(7) . 74_565 ?
O3 Ga2 Ca2 100.1(2) . 74_565 ?
O3 Ga2 Ca2 71.3(2) 6_566 74_565 ?
O3 Ga2 Ca2 139.4(2) 12_665 74_565 ?
Ca1 Ga2 Ca2 62.24(6) 74_565 74_565 ?
Ca1 Ga2 Ca2 62.23(6) . 74_565 ?
Ca1 Ga2 Ca2 119.15(10) 51 74_565 ?
Ca2 Ga2 Ca2 68.24(12) 51 74_565 ?
O2 Ga2 Ca2 40.37(7) . 28_565 ?
O3 Ga2 Ca2 139.4(2) . 28_565 ?
O3 Ga2 Ca2 100.1(2) 6_566 28_565 ?
O3 Ga2 Ca2 71.3(2) 12_665 28_565 ?
Ca1 Ga2 Ca2 62.24(6) 74_565 28_565 ?
Ca1 Ga2 Ca2 119.15(10) . 28_565 ?
Ca1 Ga2 Ca2 62.23(6) 51 28_565 ?
Ca2 Ga2 Ca2 68.24(12) 51 28_565 ?
Ca2 Ga2 Ca2 68.24(12) 74_565 28_565 ?
O3 Ga3 O3 107.5(6) . 72_575 ?
O3 Ga3 O3 109.0(5) . 22_575 ?
O3 Ga3 O3 111.9(5) 72_575 22_575 ?
O3 Ga3 O3 111.9(5) . 51 ?
O3 Ga3 O3 109.0(5) 72_575 51 ?
O3 Ga3 O3 107.5(6) 22_575 51 ?
O3 Ga3 Ca2 36.7(3) . . ?
O3 Ga3 Ca2 143.3(3) 72_575 . ?
O3 Ga3 Ca2 93.0(3) 22_575 . ?
O3 Ga3 Ca2 87.0(3) 51 . ?
O3 Ga3 Ca2 143.3(3) . 61_465 ?
O3 Ga3 Ca2 36.7(3) 72_575 61_465 ?
O3 Ga3 Ca2 87.0(3) 22_575 61_465 ?
O3 Ga3 Ca2 93.0(3) 51 61_465 ?
Ca2 Ga3 Ca2 180.0(2) . 61_465 ?
O3 Ga3 Ca2 93.0(3) . 16_665 ?
O3 Ga3 Ca2 87.0(3) 72_575 16_665 ?
O3 Ga3 Ca2 36.7(3) 22_575 16_665 ?
O3 Ga3 Ca2 143.3(3) 51 16_665 ?
Ca2 Ga3 Ca2 99.5(4) . 16_665 ?
Ca2 Ga3 Ca2 80.5(4) 61_465 16_665 ?
O3 Ga3 Ca2 87.0(3) . 51 ?
O3 Ga3 Ca2 93.0(3) 72_575 51 ?
O3 Ga3 Ca2 143.3(3) 22_575 51 ?
O3 Ga3 Ca2 36.7(3) 51 51 ?
Ca2 Ga3 Ca2 80.5(4) . 51 ?
Ca2 Ga3 Ca2 99.5(4) 61_465 51 ?
Ca2 Ga3 Ca2 180 16_665 51 ?
O3 Ga3 Ca1 104.1(3) . 51 ?
O3 Ga3 Ca1 142.1(3) 72_575 51 ?
O3 Ga3 Ca1 75.9(3) 22_575 51 ?
O3 Ga3 Ca1 37.9(3) 51 51 ?
Ca2 Ga3 Ca1 68.13(7) . 51 ?
Ca2 Ga3 Ca1 111.87(7) 61_465 51 ?
Ca2 Ga3 Ca1 111.87(7) 16_665 51 ?
Ca2 Ga3 Ca1 68.13(7) 51 51 ?
O3 Ga3 Ca1 75.9(3) . 87_465 ?
O3 Ga3 Ca1 37.9(3) 72_575 87_465 ?
O3 Ga3 Ca1 104.1(3) 22_575 87_465 ?
O3 Ga3 Ca1 142.1(3) 51 87_465 ?
Ca2 Ga3 Ca1 111.87(7) . 87_465 ?
Ca2 Ga3 Ca1 68.13(7) 61_465 87_465 ?
Ca2 Ga3 Ca1 68.13(7) 16_665 87_465 ?
Ca2 Ga3 Ca1 111.87(7) 51 87_465 ?
Ca1 Ga3 Ca1 180.00(4) 51 87_465 ?
O3 Ga3 Ca1 142.1(3) . 38_665 ?
O3 Ga3 Ca1 104.1(3) 72_575 38_665 ?
O3 Ga3 Ca1 37.9(3) 22_575 38_665 ?
O3 Ga3 Ca1 75.9(3) 51 38_665 ?
Ca2 Ga3 Ca1 111.87(7) . 38_665 ?
Ca2 Ga3 Ca1 68.13(7) 61_465 38_665 ?
Ca2 Ga3 Ca1 68.13(7) 16_665 38_665 ?
Ca2 Ga3 Ca1 111.87(7) 51 38_665 ?
Ca1 Ga3 Ca1 58.43(6) 51 38_665 ?
Ca1 Ga3 Ca1 121.57(6) 87_465 38_665 ?
O3 Ga3 Ca1 37.9(3) . . ?
O3 Ga3 Ca1 75.9(3) 72_575 . ?
O3 Ga3 Ca1 142.1(3) 22_575 . ?
O3 Ga3 Ca1 104.1(3) 51 . ?
Ca2 Ga3 Ca1 68.13(7) . . ?
Ca2 Ga3 Ca1 111.87(7) 61_465 . ?
Ca2 Ga3 Ca1 111.87(7) 16_665 . ?
Ca2 Ga3 Ca1 68.13(7) 51 . ?
Ca1 Ga3 Ca1 121.57(6) 51 . ?
Ca1 Ga3 Ca1 58.43(6) 87_465 . ?
Ca1 Ga3 Ca1 180 38_665 . ?
O4 Ga4 O4 180 16_665 3 ?
O4 Ga4 O4 109.5 16_665 15_465 ?
O4 Ga4 O4 70.529(3) 3 15_465 ?
O4 Ga4 O4 109.471(4) 16_665 14_665 ?
O4 Ga4 O4 70.5 3 14_665 ?
O4 Ga4 O4 109.4710(10) 15_465 14_665 ?
O4 Ga4 O4 109.4710(10) 16_665 13_465 ?
O4 Ga4 O4 70.529(3) 3 13_465 ?
O4 Ga4 O4 109.4710(10) 15_465 13_465 ?
O4 Ga4 O4 109.4710(10) 14_665 13_465 ?
O4 Ga4 O4 70.5 16_665 4_575 ?
O4 Ga4 O4 109.4710(10) 3 4_575 ?
O4 Ga4 O4 180 15_465 4_575 ?
O4 Ga4 O4 70.5 14_665 4_575 ?
O4 Ga4 O4 70.5290(10) 13_465 4_575 ?
O4 Ga4 O4 70.529(2) 16_665 2_575 ?
O4 Ga4 O4 109.4710(10) 3 2_575 ?
O4 Ga4 O4 70.529(2) 15_465 2_575 ?
O4 Ga4 O4 180 14_665 2_575 ?
O4 Ga4 O4 70.529(3) 13_465 2_575 ?
O4 Ga4 O4 109.4710(10) 4_575 2_575 ?
O4 Ga4 O4 70.5 16_665 . ?
O4 Ga4 O4 109.4710(10) 3 . ?
O4 Ga4 O4 70.5 15_465 . ?
O4 Ga4 O4 70.5 14_665 . ?
O4 Ga4 O4 180 13_465 . ?
O4 Ga4 O4 109.471(4) 4_575 . ?
O4 Ga4 O4 109.4710(10) 2_575 . ?
O4 Ga4 Sr1 125.2640(10) 16_665 2_575 ?
O4 Ga4 Sr1 54.7 3 2_575 ?
O4 Ga4 Sr1 54.7 15_465 2_575 ?
O4 Ga4 Sr1 125.2640(10) 14_665 2_575 ?
O4 Ga4 Sr1 54.7360(10) 13_465 2_575 ?
O4 Ga4 Sr1 125.2640(10) 4_575 2_575 ?
O4 Ga4 Sr1 54.7360(10) 2_575 2_575 ?
O4 Ga4 Sr1 125.2640(10) . 2_575 ?
O4 Ga4 Sr1 125.3 16_665 10_665 ?
O4 Ga4 Sr1 54.7360(10) 3 10_665 ?
O4 Ga4 Sr1 125.2640(10) 15_465 10_665 ?
O4 Ga4 Sr1 54.7 14_665 10_665 ?
O4 Ga4 Sr1 54.7360(10) 13_465 10_665 ?
O4 Ga4 Sr1 54.7 4_575 10_665 ?
O4 Ga4 Sr1 125.2640(10) 2_575 10_665 ?
O4 Ga4 Sr1 125.3 . 10_665 ?
Sr1 Ga4 Sr1 90 2_575 10_665 ?
O4 Ga4 Sr1 54.7 16_665 9_465 ?
O4 Ga4 Sr1 125.3 3 9_465 ?
O4 Ga4 Sr1 54.7360(10) 15_465 9_465 ?
O4 Ga4 Sr1 125.3 14_665 9_465 ?
O4 Ga4 Sr1 125.2640(10) 13_465 9_465 ?
O4 Ga4 Sr1 125.3 4_575 9_465 ?
O4 Ga4 Sr1 54.7360(10) 2_575 9_465 ?
O4 Ga4 Sr1 54.7 . 9_465 ?
Sr1 Ga4 Sr1 90 2_575 9_465 ?
Sr1 Ga4 Sr1 180 10_665 9_465 ?
O4 Ga4 Sr1 125.2640(10) 16_665 6_566 ?
O4 Ga4 Sr1 54.7360(10) 3 6_566 ?
O4 Ga4 Sr1 54.7360(10) 15_465 6_566 ?
O4 Ga4 Sr1 54.7 14_665 6_566 ?
O4 Ga4 Sr1 125.2640(10) 13_465 6_566 ?
O4 Ga4 Sr1 125.2640(10) 4_575 6_566 ?
O4 Ga4 Sr1 125.2640(10) 2_575 6_566 ?
O4 Ga4 Sr1 54.7 . 6_566 ?
Sr1 Ga4 Sr1 90 2_575 6_566 ?
Sr1 Ga4 Sr1 90 10_665 6_566 ?
Sr1 Ga4 Sr1 90 9_465 6_566 ?
O3 Ca1 O3 95.5(3) 80_556 59_465 ?
O3 Ca1 O3 95.5(3) 80_556 . ?
O3 Ca1 O3 95.5(3) 59_465 . ?
O3 Ca1 O1 149.8(2) 80_556 58_665 ?
O3 Ca1 O1 84.2(3) 59_465 58_665 ?
O3 Ca1 O1 114.6(2) . 58_665 ?
O3 Ca1 O1 84.2(3) 80_556 77_554 ?
O3 Ca1 O1 114.6(2) 59_465 77_554 ?
O3 Ca1 O1 149.8(2) . 77_554 ?
O1 Ca1 O1 68.8(3) 58_665 77_554 ?
O3 Ca1 O1 114.6(2) 80_556 . ?
O3 Ca1 O1 149.8(2) 59_465 . ?
O3 Ca1 O1 84.2(3) . . ?
O1 Ca1 O1 68.8(3) 58_665 . ?
O1 Ca1 O1 68.8(3) 77_554 . ?
O3 Ca1 Ga1 121.3(2) 80_556 . ?
O3 Ca1 Ga1 121.3(2) 59_465 . ?
O3 Ca1 Ga1 121.3(2) . . ?
O1 Ca1 Ga1 40.7(2) 58_665 . ?
O1 Ca1 Ga1 40.7(2) 77_554 . ?
O1 Ca1 Ga1 40.7(2) . . ?
O3 Ca1 Mn1 121.3(2) 80_556 . ?
O3 Ca1 Mn1 121.3(2) 59_465 . ?
O3 Ca1 Mn1 121.3(2) . . ?
O1 Ca1 Mn1 40.7(2) 58_665 . ?
O1 Ca1 Mn1 40.7(2) 77_554 . ?
O1 Ca1 Mn1 40.7(2) . . ?
Ga1 Ca1 Mn1 0 . . ?
O3 Ca1 Ca1 105.72(17) 80_556 88_655 ?
O3 Ca1 Ca1 73.2(2) 59_465 88_655 ?
O3 Ca1 Ca1 156.6(2) . 88_655 ?
O1 Ca1 Ca1 45.26(2) 58_665 88_655 ?
O1 Ca1 Ca1 45.26(2) 77_554 88_655 ?
O1 Ca1 Ca1 95.5(2) . 88_655 ?
Ga1 Ca1 Ca1 54.7 . 88_655 ?
Mn1 Ca1 Ca1 54.7 . 88_655 ?
O3 Ca1 Ca1 156.6(2) 80_556 87_465 ?
O3 Ca1 Ca1 105.72(17) 59_465 87_465 ?
O3 Ca1 Ca1 73.2(2) . 87_465 ?
O1 Ca1 Ca1 45.26(2) 58_665 87_465 ?
O1 Ca1 Ca1 95.5(2) 77_554 87_465 ?
O1 Ca1 Ca1 45.262(19) . 87_465 ?
Ga1 Ca1 Ca1 54.7 . 87_465 ?
Mn1 Ca1 Ca1 54.7 . 87_465 ?
Ca1 Ca1 Ca1 90 88_655 87_465 ?
O3 Ca1 Ca1 73.2(2) 80_556 85_455 ?
O3 Ca1 Ca1 156.6(2) 59_465 85_455 ?
O3 Ca1 Ca1 105.72(17) . 85_455 ?
O1 Ca1 Ca1 95.5(2) 58_665 85_455 ?
O1 Ca1 Ca1 45.26(2) 77_554 85_455 ?
O1 Ca1 Ca1 45.262(19) . 85_455 ?
Ga1 Ca1 Ca1 54.7 . 85_455 ?
Mn1 Ca1 Ca1 54.7 . 85_455 ?
Ca1 Ca1 Ca1 90 88_655 85_455 ?
Ca1 Ca1 Ca1 90 87_465 85_455 ?
O3 Ca1 Ga3 28.9(2) 80_556 6_566 ?
O3 Ca1 Ga3 117.36(19) 59_465 6_566 ?
O3 Ca1 Ga3 75.2(2) . 6_566 ?
O1 Ca1 Ga3 156.3(2) 58_665 6_566 ?
O1 Ca1 Ga3 91.83(13) 77_554 6_566 ?
O1 Ca1 Ga3 91.82(13) . 6_566 ?
Ga1 Ca1 Ga3 115.52(3) . 6_566 ?
Mn1 Ca1 Ga3 115.52(3) . 6_566 ?
Ca1 Ca1 Ga3 128.109(14) 88_655 6_566 ?
Ca1 Ca1 Ga3 128.109(14) 87_465 6_566 ?
Ca1 Ca1 Ga3 60.78(3) 85_455 6_566 ?
O3 Ca2 O3 119.9990(10) . 12_665 ?
O3 Ca2 O3 120.001(2) . 6_566 ?
O3 Ca2 O3 120.0000(10) 12_665 6_566 ?
O3 Ca2 O4 89.9(4) . . ?
O3 Ca2 O4 89.9(4) 12_665 . ?
O3 Ca2 O4 89.9(4) 6_566 . ?
O3 Ca2 O2 90.1(4) . . ?
O3 Ca2 O2 90.1(4) 12_665 . ?
O3 Ca2 O2 90.1(4) 6_566 . ?
O4 Ca2 O2 180.0(8) . . ?
O3 Ca2 Ga3 33.02(19) . . ?
O3 Ca2 Ga3 87.3(2) 12_665 . ?
O3 Ca2 Ga3 152.3(2) 6_566 . ?
O4 Ca2 Ga3 95.0(2) . . ?
O2 Ca2 Ga3 85.0(2) . . ?
O3 Ca2 Ga3 152.3(2) . 34_655 ?
O3 Ca2 Ga3 33.02(19) 12_665 34_655 ?
O3 Ca2 Ga3 87.3(2) 6_566 34_655 ?
O4 Ca2 Ga3 95.0(2) . 34_655 ?
O2 Ca2 Ga3 85.0(2) . 34_655 ?
Ga3 Ca2 Ga3 119.25(6) . 34_655 ?
O3 Ca2 Ga3 87.3(2) . 6_566 ?
O3 Ca2 Ga3 152.3(2) 12_665 6_566 ?
O3 Ca2 Ga3 33.02(19) 6_566 6_566 ?
O4 Ca2 Ga3 95.0(2) . 6_566 ?
O2 Ca2 Ga3 85.0(2) . 6_566 ?
Ga3 Ca2 Ga3 119.25(6) . 6_566 ?
Ga3 Ca2 Ga3 119.25(6) 34_655 6_566 ?
O3 Ca2 Sr1 92.0(3) . 9_465 ?
O3 Ca2 Sr1 48.2(3) 12_665 9_465 ?
O3 Ca2 Sr1 129.1(4) 6_566 9_465 ?
O4 Ca2 Sr1 48.60(14) . 9_465 ?
O2 Ca2 Sr1 131.40(14) . 9_465 ?
Ga3 Ca2 Sr1 71.57(9) . 9_465 ?
Ga3 Ca2 Sr1 71.57(9) 34_655 9_465 ?
Ga3 Ca2 Sr1 143.6(3) 6_566 9_465 ?
O3 Ca2 Sr1 129.1(4) . 6_566 ?
O3 Ca2 Sr1 92.0(3) 12_665 6_566 ?
O3 Ca2 Sr1 48.2(3) 6_566 6_566 ?
O4 Ca2 Sr1 48.60(14) . 6_566 ?
O2 Ca2 Sr1 131.40(14) . 6_566 ?
Ga3 Ca2 Sr1 143.6(3) . 6_566 ?
Ga3 Ca2 Sr1 71.57(9) 34_655 6_566 ?
Ga3 Ca2 Sr1 71.57(9) 6_566 6_566 ?
Sr1 Ca2 Sr1 81.0(2) 9_465 6_566 ?
O3 Ca2 Sr1 48.2(3) . . ?
O3 Ca2 Sr1 129.1(4) 12_665 . ?
O3 Ca2 Sr1 92.0(3) 6_566 . ?
O4 Ca2 Sr1 48.60(14) . . ?
O2 Ca2 Sr1 131.40(14) . . ?
Ga3 Ca2 Sr1 71.57(9) . . ?
Ga3 Ca2 Sr1 143.6(3) 34_655 . ?
Ga3 Ca2 Sr1 71.57(9) 6_566 . ?
Sr1 Ca2 Sr1 81.0(2) 9_465 . ?
Sr1 Ca2 Sr1 81.0(2) 6_566 . ?
O3 Ca2 Ga2 65.0(3) . 51 ?
O3 Ca2 Ga2 88.7(3) 12_665 51 ?
O3 Ca2 Ga2 116.6(4) 6_566 51 ?
O4 Ca2 Ga2 149.84(7) . 51 ?
O2 Ca2 Ga2 30.16(7) . 51 ?
Ga3 Ca2 Ga2 54.85(15) . 51 ?
Ga3 Ca2 Ga2 100.1(2) 34_655 51 ?
Ga3 Ca2 Ga2 100.1(2) 6_566 51 ?
Sr1 Ca2 Ga2 112.54(8) 9_465 51 ?
Sr1 Ca2 Ga2 161.6(2) 6_566 51 ?
Sr1 Ca2 Ga2 112.54(8) . 51 ?
Mn1 O1 Ga1 0 . . ?
Mn1 O1 Ca1 84.5(2) . 87_465 ?
Ga1 O1 Ca1 84.5(2) . 87_465 ?
Mn1 O1 Ca1 84.5(2) . 85_455 ?
Ga1 O1 Ca1 84.5(2) . 85_455 ?
Ca1 O1 Ca1 169.0(4) 87_465 85_455 ?
Mn1 O1 Ca1 84.5(2) . . ?
Ga1 O1 Ca1 84.5(2) . . ?
Ca1 O1 Ca1 89.48(4) 87_465 . ?
Ca1 O1 Ca1 89.48(4) 85_455 . ?
Mn1 O1 Ca1 84.5(2) . 4_575 ?
Ga1 O1 Ca1 84.5(2) . 4_575 ?
Ca1 O1 Ca1 89.48(4) 87_465 4_575 ?
Ca1 O1 Ca1 89.48(4) 85_455 4_575 ?
Ca1 O1 Ca1 169.0(4) . 4_575 ?
Mn1 O1 Sr1 180 . . ?
Ga1 O1 Sr1 180 . . ?
Ca1 O1 Sr1 95.5(2) 87_465 . ?
Ca1 O1 Sr1 95.5(2) 85_455 . ?
Ca1 O1 Sr1 95.5(2) . . ?
Ca1 O1 Sr1 95.5(2) 4_575 . ?
Ga2 O2 Ga2 109.4710(10) . 51 ?
Ga2 O2 Ga2 109.5 . 28_565 ?
Ga2 O2 Ga2 109.5 51 28_565 ?
Ga2 O2 Ga2 109.5 . 74_565 ?
Ga2 O2 Ga2 109.4710(10) 51 74_565 ?
Ga2 O2 Ga2 109.5 28_565 74_565 ?
Ga2 O2 Ca2 0.00(10) . . ?
Ga2 O2 Ca2 109.4710(10) 51 . ?
Ga2 O2 Ca2 109.4710(10) 28_565 . ?
Ga2 O2 Ca2 109.5 74_565 . ?
Ga2 O2 Ca2 109.4710(10) . 51 ?
Ga2 O2 Ca2 0.00(17) 51 51 ?
Ga2 O2 Ca2 109.4710(10) 28_565 51 ?
Ga2 O2 Ca2 109.4710(10) 74_565 51 ?
Ca2 O2 Ca2 109.4710(10) . 51 ?
Ga2 O2 Ca2 109.4710(10) . 28_565 ?
Ga2 O2 Ca2 109.5 51 28_565 ?
Ga2 O2 Ca2 0.00(10) 28_565 28_565 ?
Ga2 O2 Ca2 109.5 74_565 28_565 ?
Ca2 O2 Ca2 109.4710(10) . 28_565 ?
Ca2 O2 Ca2 109.5 51 28_565 ?
Ga2 O2 Ca2 109.5 . 74_565 ?
Ga2 O2 Ca2 109.4710(10) 51 74_565 ?
Ga2 O2 Ca2 109.5 28_565 74_565 ?
Ga2 O2 Ca2 0.00(17) 74_565 74_565 ?
Ca2 O2 Ca2 109.5 . 74_565 ?
Ca2 O2 Ca2 109.471(2) 51 74_565 ?
Ca2 O2 Ca2 109.5 28_565 74_565 ?
Ga3 O3 Ca2 110.3(4) . . ?
Ga3 O3 Ga2 107.1(4) . . ?
Ca2 O3 Ga2 15.6(3) . . ?
Ga3 O3 Ca1 113.2(4) . . ?
Ca2 O3 Ca1 118.5(4) . . ?
Ga2 O3 Ca1 108.3(3) . . ?
Ga3 O3 Sr1 121.0(4) . . ?
Ca2 O3 Sr1 97.1(4) . . ?
Ga2 O3 Sr1 110.8(4) . . ?
Ca1 O3 Sr1 95.7(3) . . ?
Ga4 O4 Ca2 180.0(13) . . ?
Ga4 O4 Sr1 90.9(4) . 6_566 ?
Ca2 O4 Sr1 89.1(4) . 6_566 ?
Ga4 O4 Sr1 90.9(4) . 9_465 ?
Ca2 O4 Sr1 89.1(4) . 9_465 ?
Sr1 O4 Sr1 119.978(19) 6_566 9_465 ?
Ga4 O4 Sr1 90.9(4) . . ?
Ca2 O4 Sr1 89.1(4) . . ?
Sr1 O4 Sr1 119.978(19) 6_566 . ?
Sr1 O4 Sr1 119.978(19) 9_465 . ?



# END of CIF
